Comparative study of the interfaces of graphene and hexagonal boron nitride Ir(111)  and for...
Embed Size (px)
Transcript of Comparative study of the interfaces of graphene and hexagonal boron nitride Ir(111)  and for...
General rights Copyright and moral rights for the publications made accessible in the public portal are retained by the authors and/or other copyright owners and it is a condition of accessing publications that users recognise and abide by the legal requirements associated with these rights.
Users may download and print one copy of any publication from the public portal for the purpose of private study or research.
You may not further distribute the material or use it for any profit-making activity or commercial gain
You may freely distribute the URL identifying the publication in the public portal If you believe that this document breaches copyright please contact us providing details, and we will remove access to the work immediately and investigate your claim.
Downloaded from orbit.dtu.dk on: Aug 13, 2021
Comparative study of the interfaces of graphene and hexagonal boron nitride with silver
Garnica, Manuela; Schwarz, Martin; Ducke, Jacob; He, Yuanqin; Bischoff, Felix; Barth, Johannes V.; Auwarter, Willi; Stradi, Daniele
Published in: Physical Review B
Link to article, DOI: 10.1103/PhysRevB.94.155431
Publication date: 2016
Document Version Publisher's PDF, also known as Version of record
Link back to DTU Orbit
Citation (APA): Garnica, M., Schwarz, M., Ducke, J., He, Y., Bischoff, F., Barth, J. V., Auwarter, W., & Stradi, D. (2016). Comparative study of the interfaces of graphene and hexagonal boron nitride with silver. Physical Review B, 94(15), . https://doi.org/10.1103/PhysRevB.94.155431
https://doi.org/10.1103/PhysRevB.94.155431 https://orbit.dtu.dk/en/publications/40c5f49d-af78-4300-9f9b-03d46fb9382c https://doi.org/10.1103/PhysRevB.94.155431
PHYSICAL REVIEW B 94, 155431 (2016)
Comparative study of the interfaces of graphene and hexagonal boron nitride with silver
Manuela Garnica,* Martin Schwarz, Jacob Ducke, Yuanqin He, Felix Bischoff, Johannes V. Barth, and Willi Auwärter
Physik-Department E20, Technische Universität München, James-Franck-Strasse 1, 85748 Garching, Germany
Daniele Stradi Department of Micro- and Nanotechnology, Center for Nanostructured Graphene, Technical University of Denmark,
DK-2800 Kgs. Lyngby, Denmark (Received 23 May 2016; revised manuscript received 19 August 2016; published 18 October 2016)
Silver opens up interesting perspectives in the fabrication of complex systems based on heteroepitaxial layers after the growth of a silicene layer on its (111) face has been proposed. In this work we explore different synthesis methods of hexagonal boron nitride (h-BN) and graphene sheets on silver. The resulting layers have been examined by high-resolution scanning tunneling microscopy. A comparison of the interfacial electronic band structure upon growth of the distinct two-dimensional (2D) layers has been performed by scanning tunneling spectroscopy and complementary first-principle calculations. We demonstrate that the adsorption of the 2D layers has an effect on the binding energy of the Shockley state and the surface potential by lowering the local work function. These effects are larger in the case of graphene where the surface state of Ag(111) is depopulated due to charge transfer to the graphene. Furthermore, we show that the electronic properties of the h-BN/silver system can be tuned by employing different thicknesses of silver ranging from a few monolayers on Cu(111) to the single crystal Ag substrate.
In recent years, silver surfaces emerged as a promising platform for the synthesis of atomically thin materials after the growth of silicene has been proposed , which presents potential advantages for future device applications . The synthesis and investigation of other 2D materials on Ag(111) at the atomic scale opens up possibilities to design 2D het- erostructures that can provide access to fundamental physics and an improved flexibility to realize devices . As an initial step for these potential applications, a reliable synthesis of single- and few-layer 2D materials becomes crucial. In particular, the chemical vapor deposition (CVD) technique has been shown advantageous to fabricate ultrathin, large-scale graphene and h-BN sheets on reactive metals like Ru, Rh, Ir, Co, Ni and Pd [4–8]. However, the low catalytic activity of noble metals as Ag and Au impairs the growth of graphene  and h-BN [10,11] by standard CVD procedures. As an alternative method, atomic deposition has been successfully used for the growth of graphene [12,13]. However, the synthesis of h-BN on silver is still challenging .
The pertaining interfaces are of great interest and impor- tance. We can classify them depending on the interaction strength between the 2D layer and the metal . Silver is considered a weakly interacting system where the electronic properties of both the 2D layer and the silver substrate would remain practically unperturbed. In particular, a unique feature of the close-packed surfaces of noble metals is the presence of a surface state with nearly free electron gas characteristics. Scanning tunneling microscopy (STM) is a powerful tool to probe these states, which are confined in perpendicular direc- tion to the surfaces. Relevant and quantitative information can
be extracted from the study of the evolution and modification of these states by the adsorption of gases [14–16], molecules [17–22], ionic films , and 2D honeycomb layers [24–26]. On the other hand, scanning tunneling spectroscopy (STS) has been exploited to investigate the unoccupied states of ultrathin layers on metals, in particular, the image potential states [24,27–29]. They are bound to a solid by the response of the substrate to the presence of the electron and kept outside the surface by the reflective properties of the substrate. Experimentally, one can access these states in the field- emission regime by STS and they are thus known as field emission resonances (FERs) . The evolution of the FERs can provide quantitative information on changes in the local electrostatic surface potential which manifest as local work function variation. In this work we present an investigation of the modification of the surface states on the (111) face of a silver crystal after the growth of graphene and boron nitride yielding information about the interfaces. We track back the modification of the Shockley-type surface state to charge transfer and local work function modifications upon the formation of the 2D layers.
The experiments were performed in a custom-designed ultrahigh vacuum (UHV) system, equipped with a commercial low-temperature CreaTec STM. The base pressure was below 2 × 10−10 mbar. The Ag(111) single crystal surface was prepared by several cycles consisting of sputtering by a 800 eV Ar+ ion beam followed by annealing at 900 K. All STM images were taken at 5 K in constant-current mode and the differential conductance (dI/dV ) spectra were recorded using a lock-in amplifier (f = 969 Hz, �Vrms = 18 mV). We measured the FERs with the feedback loop connected at a current setpoint
2469-9950/2016/94(15)/155431(6) 155431-1 ©2016 American Physical Society
MANUELA GARNICA et al. PHYSICAL REVIEW B 94, 155431 (2016)
of 0.8 nA. The STM images were processed using the WSxM software .
The simulations of graphene and h-BN on Ag(111) were performed using density functional theory (DFT) as imple- mented in SIESTA . The electronic exchange-correlation energy was described using the Perdew-Burke-Ernzerhof (PBE) functional . The ionic cores were described by Trullier-Martins pseudopotentials . The real-space grid was set to a plane-wave equivalent of 200 Ry. The one-electron Kohn-Sham orbitals were expanded in a basis of double- ζ numerical atomic orbitals (NAOs) including polarization functions. The NAOs confinement radii rc of the B, C, and N s (p) shells were set to 5.16 (6.30), 4.41 (5.38), and 3.97 Å (4.73 Å), respectively. For Ag, the confinement radii for the s (d) shells were set to 5.37 Å (5.97 Å), and an additional set of s-like diffuse functions (rc = 9.0 Å) was added to the topmost layer basis set to account correctly for the electronic properties of the Ag(111) surface . The graphene/Ag(111) (h-BN/Ag(111)) system was simulated by using a 27-layer symmetric Ag slab, with the graphene (h-BN) placed at both sides of the slab. The mismatch between the graphene (h-BN) and the Ag(111) surface was accounted for by matching a 2 × 2 graphene (h-BN) supercell to a √3 × √3 Ag(111) supercell [36,37]. The resulting Brillouin zone was sampled using a Monkhorst-Pack  regular grid of 24 × 24 × 1 k points, and the electronic occupancies were determined using a Fermi-Dirac smearing of 25 meV.
A. Synthesis of 2D layers on silver
Submonolayer coverages of h-BN were prepared by ther- mal decomposition of borazine (HBNH)3 (Katchem, Czech Republic) assisted by an ion gun. The ion gun used in the standard surface preparation in UHV is used to create a beam of ionized precursors which is accelerated towards the hot sample . This procedure enhances the thermal decomposition of the precursor compared to a normal CVD procedure and allows us to grow patches of h-BN even at moderate temperatures. Figure 1(a) shows an STM image
recorded after exposing the Ag substrate at 900 K to 2700 L of borazine using a beam energy of 300 eV. The structural quality of the h-BN islands is highlighted by the inset of Fig. 1(a). At this particular setpoint the at